#------------------------------------------------------------------------------
#$Date: 2019-11-17 09:37:40 +0200 (Sun, 17 Nov 2019) $
#$Revision: 229146 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/00/7230087.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7230087
loop_
_publ_author_name
'Tian, Xuerui'
'Xin, Xing'
'Gao, Yuanzhe'
'Han, Zhangang'
_publ_section_title
;
 Supramolecular cooperative interaction-induced assembly of
 phosphotungstate polyanions and sulfur-containing pyridine-based cations
;
_journal_issue                   11
_journal_name_full               CrystEngComm
_journal_page_first              1588
_journal_paper_doi               10.1039/C8CE00026C
_journal_volume                  20
_journal_year                    2018
_chemical_formula_sum            'C20 H48 Ag12 N4 O137 P4 S4 W36'
_chemical_formula_weight         10701.46
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2017-12-26 deposited with the CCDC.
2018-02-07 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 120.559(5)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.9281(17)
_cell_length_b                   20.076(2)
_cell_length_c                   26.708(3)
_cell_measurement_reflns_used    3135
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      26.80
_cell_measurement_theta_min      2.51
_cell_volume                     6892.5(13)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.975
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0817
_diffrn_reflns_av_unetI/netI     0.0939
_diffrn_reflns_Laue_measured_fraction_full 0.975
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            34429
_diffrn_reflns_point_group_measured_fraction_full 0.975
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.010
_diffrn_reflns_theta_min         1.346
_exptl_absorpt_coefficient_mu    31.782
_exptl_absorpt_correction_T_max  0.009
_exptl_absorpt_correction_T_min  0.002
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    5.156
_exptl_crystal_description       block
_exptl_crystal_F_000             9284
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.15
_refine_diff_density_max         4.035
_refine_diff_density_min         -5.325
_refine_diff_density_rms         0.550
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     976
_refine_ls_number_reflns         12137
_refine_ls_number_restraints     2136
_refine_ls_restrained_S_all      0.979
_refine_ls_R_factor_all          0.0966
_refine_ls_R_factor_gt           0.0533
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0669P)²+27.0255P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1297
_refine_ls_wR_factor_ref         0.1565
_reflns_Friedel_coverage         0.000
_reflns_number_gt                7719
_reflns_number_total             12137
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c8ce00026c2.cif
_cod_data_source_block           286
_cod_depositor_comments
'Adding full bibliography for 7230085--7230087.cif.'
_cod_database_code               7230087
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014-3
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
W1 W 0.67305(9) 0.08050(5) 0.26316(5) 0.0177(3) Uani 1 1 d . . .
W2 W 0.42727(9) 0.17590(5) 0.19778(5) 0.0216(3) Uani 1 1 d . . .
W3 W 0.50190(9) 0.25266(5) 0.32511(5) 0.0194(3) Uani 1 1 d . . .
W4 W 0.43702(9) 0.34554(5) 0.20572(5) 0.0198(3) Uani 1 1 d . . .
W5 W 0.74786(9) 0.15708(5) 0.39041(5) 0.0157(2) Uani 1 1 d . . .
W6 W 0.59391(9) 0.18176(5) 0.13194(5) 0.0202(3) Uani 1 1 d . . .
W7 W 0.69053(9) 0.43186(5) 0.28153(5) 0.0179(3) Uani 1 1 d . . .
W8 W 0.60676(9) 0.34834(5) 0.14126(5) 0.0183(3) Uani 1 1 d . . .
W9 W 0.75734(9) 0.33932(5) 0.40027(5) 0.0172(3) Uani 1 1 d . . .
W10 W 1.03356(9) 0.33701(5) 0.43179(5) 0.0178(3) Uani 1 1 d . . .
W11 W 0.96464(9) 0.42919(5) 0.31235(5) 0.0177(3) Uani 1 1 d . . .
W12 W 0.88121(9) 0.34630(5) 0.17301(5) 0.0174(2) Uani 1 1 d . . .
W13 W 1.15670(9) 0.33918(5) 0.28863(5) 0.0208(3) Uani 1 1 d . . .
W14 W 1.14601(9) 0.17068(5) 0.27810(5) 0.0221(3) Uani 1 1 d . . .
W15 W 0.86938(9) 0.17869(5) 0.16287(5) 0.0193(3) Uani 1 1 d . . .
W16 W 0.94737(9) 0.07787(5) 0.29379(5) 0.0178(3) Uani 1 1 d . . .
W17 W 1.22724(9) 0.24574(5) 0.40843(5) 0.0211(3) Uani 1 1 d . . .
W18 W 1.02310(9) 0.15418(5) 0.42112(5) 0.0164(2) Uani 1 1 d . . .
P1 P 0.6701(5) 0.2565(3) 0.2677(3) 0.0115(14) Uani 1 1 d . . .
P2 P 0.9622(5) 0.2543(3) 0.3014(3) 0.0117(14) Uani 1 1 d . . .
Ag1 Ag 1.0000 0.0000 0.5000 0.0327(8) Uani 1 2 d S U P
Ag2 Ag 0.78517(19) -0.02661(12) 0.40748(12) 0.0415(6) Uani 1 1 d . U .
Ag3 Ag 1.13845(19) -0.02430(12) 0.45140(12) 0.0437(7) Uani 1 1 d . U .
Ag4 Ag 0.6653(3) -0.14848(16) 0.45776(16) 0.0528(10) Uani 0.75 1 d . U P
Ag5 Ag 0.5828(5) -0.0811(2) 0.1721(2) 0.0474(13) Uani 0.5 1 d . U P
Ag6 Ag 0.6558(6) -0.0822(3) 0.0533(3) 0.0722(18) Uani 0.5 1 d . U P
Ag7 Ag 0.8659(5) 0.0381(3) 0.0492(3) 0.0569(15) Uani 0.5 1 d . U P
Ag8 Ag 1.2196(5) 0.4513(3) 0.5816(3) 0.0635(17) Uani 0.5 1 d . U P
Ag9 Ag 0.4314(12) -0.1973(4) 0.0219(4) 0.185(5) Uani 0.5 1 d . U P
Ag10 Ag 0.5955(16) 0.0333(11) -0.0367(10) 0.151(7) Uani 0.25 1 d . U P
O1 O 0.6086(14) 0.1854(8) 0.3587(8) 0.020(3) Uani 1 1 d . U .
O2 O 0.6670(13) 0.2598(7) 0.2085(7) 0.0160(16) Uani 1 1 d . U .
O3 O 0.7183(14) 0.1911(7) 0.2996(7) 0.0160(16) Uani 1 1 d . U .
O4 O 0.5547(14) 0.2573(7) 0.2536(7) 0.0160(16) Uani 1 1 d . U .
O5 O 0.7259(13) 0.3162(7) 0.3061(7) 0.017(3) Uani 1 1 d . U .
O6 O 1.0774(14) 0.2531(7) 0.3136(7) 0.0155(19) Uani 1 1 d . U .
O7 O 0.8907(14) 0.2595(7) 0.2346(7) 0.0155(19) Uani 1 1 d . U .
O8 O 0.9422(14) 0.1898(7) 0.3252(8) 0.019(3) Uani 1 1 d . U .
O9 O 0.9508(14) 0.3150(7) 0.3316(7) 0.017(3) Uani 1 1 d . U .
O10 O 0.7055(14) 0.0790(8) 0.3431(8) 0.023(3) Uani 1 1 d . U .
O11 O 0.5403(14) 0.1151(8) 0.2420(8) 0.024(3) Uani 1 1 d . U .
O12 O 0.7621(15) 0.1237(8) 0.4534(8) 0.026(3) Uani 1 1 d . U .
O13 O 0.3197(15) 0.1294(8) 0.1551(8) 0.026(4) Uani 1 1 d . U .
O14 O 0.4203(14) 0.1913(7) 0.2662(7) 0.018(3) Uani 1 1 d . U .
O15 O 0.4260(14) 0.3229(8) 0.2735(8) 0.023(3) Uani 1 1 d . U .
O16 O 0.3643(15) 0.2631(8) 0.1724(8) 0.025(3) Uani 1 1 d . U .
O17 O 0.4493(15) 0.2495(8) 0.3696(8) 0.027(3) Uani 1 1 d . U .
O18 O 0.6170(14) 0.3140(8) 0.3659(8) 0.022(3) Uani 1 1 d . U .
O19 O 0.7878(14) 0.2466(8) 0.4120(8) 0.021(3) Uani 1 1 d . U .
O20 O 0.7790(15) 0.3625(8) 0.4668(8) 0.027(4) Uani 1 1 d . U .
O21 O 0.5541(14) 0.4011(8) 0.2552(8) 0.021(3) Uani 1 1 d . U .
O22 O 0.7197(14) 0.4218(8) 0.3603(8) 0.022(3) Uani 1 1 d . U .
O23 O 0.6629(14) 0.5139(8) 0.2713(8) 0.024(3) Uani 1 1 d . U .
O24 O 0.8967(14) 0.3502(8) 0.4162(8) 0.020(3) Uani 1 1 d . U .
O25 O 0.4903(14) 0.3433(8) 0.1541(8) 0.022(3) Uani 1 1 d . U .
O26 O 0.4831(14) 0.1861(8) 0.1476(8) 0.023(3) Uani 1 1 d . U .
O27 O 0.8870(14) 0.1415(8) 0.4063(8) 0.023(3) Uani 1 1 d . U .
O28 O 0.8150(14) 0.0763(8) 0.2900(8) 0.024(3) Uani 1 1 d . U .
O29 O 1.0888(15) 0.1213(8) 0.4896(8) 0.026(3) Uani 1 1 d . U .
O30 O 0.5338(15) 0.1318(9) 0.0723(8) 0.028(3) Uani 1 1 d . U .
O31 O 0.6546(15) 0.1185(9) 0.1934(8) 0.029(3) Uani 1 1 d . U .
O32 O 1.0154(14) 0.0778(8) 0.3763(8) 0.021(3) Uani 1 1 d . U .
O33 O 1.0136(15) 0.2456(8) 0.4366(8) 0.024(3) Uani 1 1 d . U .
O34 O 0.5591(15) 0.2684(8) 0.0969(8) 0.024(3) Uani 1 1 d . U .
O35 O 0.7364(14) 0.3392(8) 0.1487(8) 0.021(3) Uani 1 1 d . U .
O36 O 1.0361(15) 0.4188(8) 0.3963(8) 0.025(3) Uani 1 1 d . U .
O37 O 0.5492(15) 0.4038(8) 0.0849(8) 0.025(3) Uani 1 1 d . U .
O38 O 0.6669(14) 0.4037(8) 0.2079(7) 0.019(3) Uani 1 1 d . U .
O39 O 0.8357(14) 0.4339(8) 0.3102(7) 0.019(3) Uani 1 1 d . U .
O40 O 1.1010(16) 0.3595(9) 0.5042(8) 0.030(3) Uani 1 1 d . U .
O41 O 0.9847(15) 0.5117(8) 0.3100(8) 0.027(3) Uani 1 1 d . U .
O42 O 0.8673(16) 0.4007(9) 0.1205(8) 0.032(4) Uani 1 1 d . U .
O43 O 1.0879(14) 0.3964(8) 0.3157(8) 0.022(3) Uani 1 1 d . U .
O44 O 0.8934(14) 0.4015(8) 0.2341(8) 0.022(3) Uani 1 1 d . U .
O45 O 1.1557(14) 0.3103(8) 0.4277(8) 0.022(3) Uani 1 1 d . U .
O46 O 1.3469(15) 0.2399(8) 0.4693(9) 0.032(4) Uani 1 1 d . U .
O47 O 0.8715(15) 0.2649(8) 0.1334(7) 0.021(3) Uani 1 1 d . U .
O48 O 1.0274(15) 0.3386(8) 0.2156(8) 0.026(3) Uani 1 1 d . U .
O49 O 1.2560(15) 0.3167(8) 0.3684(8) 0.026(3) Uani 1 1 d . U .
O50 O 1.2340(15) 0.3945(9) 0.2768(9) 0.030(4) Uani 1 1 d . U .
O51 O 1.1909(15) 0.2565(8) 0.2663(8) 0.023(3) Uani 1 1 d . U .
O52 O 1.2470(14) 0.1836(8) 0.3597(8) 0.026(3) Uani 1 1 d . U .
O53 O 1.2179(15) 0.1204(8) 0.2604(8) 0.026(3) Uani 1 1 d . U .
O54 O 0.8562(16) 0.1307(9) 0.1072(9) 0.034(3) Uani 1 1 d . U .
O55 O 1.0737(14) 0.1089(8) 0.2987(8) 0.022(3) Uani 1 1 d . U .
O56 O 0.8805(15) 0.1170(8) 0.2190(8) 0.027(3) Uani 1 1 d . U .
O57 O 0.9592(15) -0.0038(9) 0.2815(8) 0.030(3) Uani 1 1 d . U .
O58 O 1.0190(14) 0.1824(8) 0.2082(8) 0.022(3) Uani 1 1 d . U .
O59 O 1.1472(14) 0.1810(8) 0.4193(8) 0.023(3) Uani 1 1 d . U .
O60 O 0.6362(15) -0.0004(8) 0.2425(9) 0.030(4) Uani 1 1 d . U .
O61 O 0.7292(15) 0.1894(8) 0.1410(8) 0.026(3) Uani 1 1 d . U .
O62 O 0.3366(14) 0.4009(8) 0.1706(8) 0.022(3) Uani 1 1 d . U .
S1 S 0.9458(6) -0.0529(3) 0.4042(3) 0.0257(16) Uani 1 1 d . . .
S2 S 0.7082(6) -0.0315(4) 0.4710(4) 0.0335(19) Uani 1 1 d . . .
C1 C 0.857(3) -0.2416(14) 0.3563(15) 0.043(5) Uani 1 1 d . U .
H1 H 0.8014 -0.2638 0.3260 0.051 Uiso 1 1 calc R U .
C2 C 0.860(2) -0.1715(14) 0.3574(14) 0.035(5) Uani 1 1 d . U .
H2 H 0.8078 -0.1465 0.3272 0.042 Uiso 1 1 calc R U .
C3 C 0.940(2) -0.1421(14) 0.4042(13) 0.030(4) Uani 1 1 d . U .
C4 C 1.022(2) -0.1794(14) 0.4481(13) 0.034(5) Uani 1 1 d . U .
H4 H 1.0804 -0.1583 0.4779 0.040 Uiso 1 1 calc R U .
C5 C 1.015(3) -0.2484(14) 0.4465(14) 0.037(5) Uani 1 1 d . U .
H5 H 1.0628 -0.2746 0.4773 0.045 Uiso 1 1 calc R U .
C6 C 0.446(2) 0.0711(13) 0.3560(14) 0.032(3) Uani 1 1 d . U .
H6 H 0.4050 0.0770 0.3160 0.038 Uiso 1 1 calc R U .
C7 C 0.534(2) 0.0287(13) 0.3827(13) 0.030(4) Uani 1 1 d . U .
H7 H 0.5498 0.0043 0.3586 0.036 Uiso 1 1 calc R U .
C8 C 0.597(2) 0.0208(14) 0.4415(14) 0.033(4) Uani 1 1 d . U .
C9 C 0.577(2) 0.0567(13) 0.4772(13) 0.031(4) Uani 1 1 d . U .
H9 H 0.6201 0.0540 0.5173 0.037 Uiso 1 1 calc R U .
C10 C 0.487(2) 0.0996(14) 0.4511(13) 0.032(3) Uani 1 1 d . U .
H10 H 0.4696 0.1249 0.4743 0.038 Uiso 1 1 calc R U .
N1 N 0.934(2) -0.2758(12) 0.3979(11) 0.033(4) Uani 1 1 d . U .
H1A H 0.9336 -0.3184 0.3942 0.040 Uiso 1 1 calc R U .
N2 N 0.4296(19) 0.1020(11) 0.3951(11) 0.033(4) Uani 1 1 d . U .
H2A H 0.3746 0.1263 0.3812 0.039 Uiso 1 1 calc R U .
O1W O 0.736(2) -0.2419(10) 0.4465(10) 0.056(5) Uani 1 1 d . U .
O2W O 0.5064(17) -0.0988(9) 0.0686(9) 0.039(2) Uani 1 1 d . U .
O3W O 0.7077(17) -0.0344(9) -0.0126(10) 0.039(2) Uani 1 1 d . U .
O4W O 0.7378(18) 0.0085(10) 0.1354(10) 0.052(3) Uani 1 1 d . U .
O5W O 0.333(4) -0.2777(17) -0.0123(16) 0.191(9) Uani 1 1 d . U .
O6W O 1.091(2) 0.4163(12) 0.6196(11) 0.065(5) Uani 1 1 d . U .
O7W O 0.0000 0.5000 0.5000 0.039(2) Uani 1 2 d S . P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O60 W1 O28 101.4(8) . .
O60 W1 O11 97.8(8) . .
O28 W1 O11 160.8(7) . .
O60 W1 O31 101.7(8) . .
O28 W1 O31 87.9(8) . .
O11 W1 O31 87.2(8) . .
O60 W1 O10 101.5(8) . .
O28 W1 O10 88.7(7) . .
O11 W1 O10 88.4(7) . .
O31 W1 O10 156.8(7) . .
O60 W1 O3 173.6(7) . .
O28 W1 O3 81.6(6) . .
O11 W1 O3 79.4(7) . .
O31 W1 O3 84.0(7) . .
O10 W1 O3 72.7(6) . .
O13 W2 O14 103.8(8) . .
O13 W2 O26 100.9(8) . .
O14 W2 O26 155.2(7) . .
O13 W2 O11 107.3(8) . .
O14 W2 O11 88.5(7) . .
O26 W2 O11 86.5(7) . .
O13 W2 O16 97.8(8) . .
O14 W2 O16 86.3(7) . .
O26 W2 O16 88.0(7) . .
O11 W2 O16 154.8(8) . .
O13 W2 O4 169.2(7) . .
O14 W2 O4 72.7(6) . .
O26 W2 O4 82.6(7) . .
O11 W2 O4 83.0(7) . .
O16 W2 O4 71.9(7) . .
O17 W3 O14 102.9(8) . .
O17 W3 O15 102.4(8) . .
O14 W3 O15 89.2(7) . .
O17 W3 O1 102.2(7) . .
O14 W3 O1 87.8(7) . .
O15 W3 O1 155.2(7) . .
O17 W3 O18 102.8(8) . .
O14 W3 O18 154.2(7) . .
O15 W3 O18 88.1(8) . .
O1 W3 O18 84.1(7) . .
O17 W3 O4 173.3(8) . .
O14 W3 O4 72.3(6) . .
O15 W3 O4 73.1(6) . .
O1 W3 O4 82.5(6) . .
O18 W3 O4 82.3(6) . .
O62 W4 O25 100.9(7) . .
O62 W4 O21 103.7(8) . .
O25 W4 O21 86.8(7) . .
O62 W4 O16 100.0(8) . .
O25 W4 O16 89.5(7) . .
O21 W4 O16 156.3(7) . .
O62 W4 O15 101.3(7) . .
O25 W4 O15 157.7(7) . .
O21 W4 O15 88.4(7) . .
O16 W4 O15 86.2(7) . .
O62 W4 O4 170.7(7) . .
O25 W4 O4 84.5(6) . .
O21 W4 O4 84.1(6) . .
O16 W4 O4 72.3(7) . .
O15 W4 O4 73.3(6) . .
O12 W5 O1 96.7(8) . .
O12 W5 O19 102.0(8) . .
O1 W5 O19 87.5(7) . .
O12 W5 O10 99.4(8) . .
O1 W5 O10 91.8(7) . .
O19 W5 O10 158.5(7) . .
O12 W5 O27 97.9(8) . .
O1 W5 O27 165.2(7) . .
O19 W5 O27 87.1(7) . .
O10 W5 O27 88.2(7) . .
O12 W5 O3 173.4(7) . .
O1 W5 O3 82.1(6) . .
O19 W5 O3 84.4(7) . .
O10 W5 O3 74.2(6) . .
O27 W5 O3 83.7(7) . .
O30 W6 O26 97.4(8) . .
O30 W6 O31 102.0(8) . .
O26 W6 O31 85.8(7) . .
O30 W6 O61 100.8(8) . .
O26 W6 O61 161.3(8) . .
O31 W6 O61 86.3(8) . .
O30 W6 O34 101.2(8) . .
O26 W6 O34 90.9(7) . .
O31 W6 O34 156.8(8) . .
O61 W6 O34 89.7(7) . .
O30 W6 O2 174.3(7) . .
O26 W6 O2 81.3(7) . .
O31 W6 O2 83.6(7) . .
O61 W6 O2 81.0(6) . .
O34 W6 O2 73.3(7) . .
O23 W7 O21 97.5(8) . .
O23 W7 O39 100.3(8) . .
O21 W7 O39 162.1(7) . .
O23 W7 O38 102.8(8) . .
O21 W7 O38 85.4(7) . .
O39 W7 O38 89.8(7) . .
O23 W7 O22 100.4(7) . .
O21 W7 O22 88.5(7) . .
O39 W7 O22 89.1(7) . .
O38 W7 O22 156.6(7) . .
O23 W7 O5 172.7(7) . .
O21 W7 O5 80.2(6) . .
O39 W7 O5 82.1(6) . .
O38 W7 O5 84.0(6) . .
O22 W7 O5 72.8(6) . .
O37 W8 O35 100.9(8) . .
O37 W8 O38 103.3(8) . .
O35 W8 O38 89.3(7) . .
O37 W8 O34 98.0(8) . .
O35 W8 O34 91.3(7) . .
O38 W8 O34 158.2(7) . .
O37 W8 O25 95.5(8) . .
O35 W8 O25 163.5(7) . .
O38 W8 O25 84.5(7) . .
O34 W8 O25 89.0(7) . .
O37 W8 O2 171.0(7) . .
O35 W8 O2 82.5(6) . .
O38 W8 O2 85.0(6) . .
O34 W8 O2 73.5(7) . .
O25 W8 O2 81.7(6) . .
O20 W9 O18 99.1(8) . .
O20 W9 O22 101.2(8) . .
O18 W9 O22 91.3(7) . .
O20 W9 O19 101.1(8) . .
O18 W9 O19 86.0(7) . .
O22 W9 O19 157.7(7) . .
O20 W9 O24 97.4(8) . .
O18 W9 O24 162.9(7) . .
O22 W9 O24 90.2(7) . .
O19 W9 O24 86.2(7) . .
O20 W9 O5 175.5(7) . .
O18 W9 O5 81.8(7) . .
O22 W9 O5 74.3(6) . .
O19 W9 O5 83.4(6) . .
O24 W9 O5 82.2(7) . .
O40 W10 O33 101.6(8) . .
O40 W10 O24 99.2(8) . .
O33 W10 O24 87.8(7) . .
O40 W10 O36 100.7(8) . .
O33 W10 O36 157.1(8) . .
O24 W10 O36 93.6(7) . .
O40 W10 O45 96.0(8) . .
O33 W10 O45 85.5(7) . .
O24 W10 O45 164.3(7) . .
O36 W10 O45 87.3(7) . .
O40 W10 O9 174.3(7) . .
O33 W10 O9 83.3(7) . .
O24 W10 O9 83.8(6) . .
O36 W10 O9 74.2(7) . .
O45 W10 O9 81.4(7) . .
O41 W11 O44 105.0(8) . .
O41 W11 O39 98.5(8) . .
O44 W11 O39 89.4(7) . .
O41 W11 O43 98.9(8) . .
O44 W11 O43 86.4(7) . .
O39 W11 O43 162.7(7) . .
O41 W11 O36 98.3(8) . .
O44 W11 O36 156.5(7) . .
O39 W11 O36 89.7(7) . .
O43 W11 O36 87.6(7) . .
O41 W11 O9 171.1(7) . .
O44 W11 O9 83.9(6) . .
O39 W11 O9 81.7(6) . .
O43 W11 O9 81.1(6) . .
O36 W11 O9 72.8(6) . .
O42 W12 O48 99.7(8) . .
O42 W12 O44 104.5(8) . .
O48 W12 O44 87.3(8) . .
O42 W12 O47 98.6(8) . .
O48 W12 O47 90.2(8) . .
O44 W12 O47 156.8(7) . .
O42 W12 O35 97.1(8) . .
O48 W12 O35 163.0(7) . .
O44 W12 O35 86.2(7) . .
O47 W12 O35 89.6(7) . .
O42 W12 O7 171.6(8) . .
O48 W12 O7 82.9(7) . .
O44 W12 O7 83.5(6) . .
O47 W12 O7 73.4(6) . .
O35 W12 O7 80.7(6) . .
O50 W13 O43 102.6(8) . .
O50 W13 O51 101.0(8) . .
O43 W13 O51 156.5(7) . .
O50 W13 O48 103.7(8) . .
O43 W13 O48 86.1(8) . .
O51 W13 O48 88.2(8) . .
O50 W13 O49 98.1(8) . .
O43 W13 O49 88.9(8) . .
O51 W13 O49 88.0(8) . .
O48 W13 O49 158.2(7) . .
O50 W13 O6 170.4(8) . .
O43 W13 O6 83.7(6) . .
O51 W13 O6 73.0(6) . .
O48 W13 O6 83.9(7) . .
O49 W13 O6 74.5(7) . .
O53 W14 O58 104.9(8) . .
O53 W14 O55 102.9(8) . .
O58 W14 O55 86.3(8) . .
O53 W14 O51 99.4(8) . .
O58 W14 O51 89.1(8) . .
O55 W14 O51 157.6(7) . .
O53 W14 O52 98.7(8) . .
O58 W14 O52 156.3(7) . .
O55 W14 O52 89.6(8) . .
O51 W14 O52 85.9(7) . .
O53 W14 O6 168.5(8) . .
O58 W14 O6 83.6(7) . .
O55 W14 O6 85.2(6) . .
O51 W14 O6 72.6(6) . .
O52 W14 O6 72.8(7) . .
O54 W15 O61 100.3(9) . .
O54 W15 O56 104.3(8) . .
O61 W15 O56 87.5(8) . .
O54 W15 O47 99.9(8) . .
O61 W15 O47 91.0(8) . .
O56 W15 O47 155.6(7) . .
O54 W15 O58 98.8(8) . .
O61 W15 O58 160.8(7) . .
O56 W15 O58 85.5(8) . .
O47 W15 O58 88.1(8) . .
O54 W15 O7 172.0(7) . .
O61 W15 O7 81.1(7) . .
O56 W15 O7 83.6(6) . .
O47 W15 O7 72.1(6) . .
O58 W15 O7 80.4(6) . .
O57 W16 O56 104.3(8) . .
O57 W16 O32 100.1(8) . .
O56 W16 O32 155.4(7) . .
O57 W16 O28 100.3(8) . .
O56 W16 O28 88.5(8) . .
O32 W16 O28 89.5(7) . .
O57 W16 O55 97.5(8) . .
O56 W16 O55 84.9(8) . .
O32 W16 O55 89.6(7) . .
O28 W16 O55 162.1(7) . .
O57 W16 O8 172.1(8) . .
O56 W16 O8 83.5(7) . .
O32 W16 O8 72.0(6) . .
O28 W16 O8 79.7(6) . .
O55 W16 O8 83.0(6) . .
O46 W17 O59 104.2(8) . .
O46 W17 O45 104.4(9) . .
O59 W17 O45 86.6(7) . .
O46 W17 O52 98.8(9) . .
O59 W17 O52 89.1(7) . .
O45 W17 O52 156.7(8) . .
O46 W17 O49 99.0(8) . .
O59 W17 O49 156.8(8) . .
O45 W17 O49 87.7(7) . .
O52 W17 O49 87.2(7) . .
O46 W17 O6 169.1(8) . .
O59 W17 O6 83.1(7) . .
O45 W17 O6 83.8(7) . .
O52 W17 O6 72.9(7) . .
O49 W17 O6 73.9(7) . .
O29 W18 O27 98.2(8) . .
O29 W18 O33 101.9(8) . .
O27 W18 O33 89.1(7) . .
O29 W18 O32 100.3(8) . .
O27 W18 O32 92.6(7) . .
O33 W18 O32 157.3(7) . .
O29 W18 O59 95.6(8) . .
O27 W18 O59 165.8(7) . .
O33 W18 O59 85.1(7) . .
O32 W18 O59 87.8(7) . .
O29 W18 O8 173.7(7) . .
O27 W18 O8 84.8(7) . .
O33 W18 O8 83.6(7) . .
O32 W18 O8 74.0(6) . .
O59 W18 O8 81.7(7) . .
O5 P1 O3 111.1(10) . .
O5 P1 O2 112.0(9) . .
O3 P1 O2 111.3(9) . .
O5 P1 O4 108.2(9) . .
O3 P1 O4 106.9(9) . .
O2 P1 O4 107.1(10) . .
O9 P2 O8 111.0(10) . .
O9 P2 O7 111.0(9) . .
O8 P2 O7 111.6(10) . .
O9 P2 O6 107.9(9) . .
O8 P2 O6 108.9(9) . .
O7 P2 O6 106.2(9) . .
S1 Ag1 S1 180.0(2) . 3_756
S1 Ag1 Ag2 54.08(18) . .
S1 Ag1 Ag2 125.92(18) 3_756 .
S1 Ag1 Ag2 125.92(18) . 3_756
S1 Ag1 Ag2 54.08(18) 3_756 3_756
Ag2 Ag1 Ag2 180.0 . 3_756
S1 Ag1 Ag3 54.56(17) . .
S1 Ag1 Ag3 125.44(17) 3_756 .
Ag2 Ag1 Ag3 107.80(7) . .
Ag2 Ag1 Ag3 72.20(7) 3_756 .
S1 Ag1 Ag3 125.44(17) . 3_756
S1 Ag1 Ag3 54.56(17) 3_756 3_756
Ag2 Ag1 Ag3 72.20(7) . 3_756
Ag2 Ag1 Ag3 107.80(7) 3_756 3_756
Ag3 Ag1 Ag3 180.0 . 3_756
O62 Ag2 S2 99.1(4) 2_645 .
O62 Ag2 S1 99.0(4) 2_645 .
S2 Ag2 S1 143.1(3) . .
O62 Ag2 O10 91.7(6) 2_645 .
S2 Ag2 O10 105.6(4) . .
S1 Ag2 O10 105.8(4) . .
O62 Ag2 Ag1 148.3(4) 2_645 .
S2 Ag2 Ag1 96.8(2) . .
S1 Ag2 Ag1 53.91(18) . .
O10 Ag2 Ag1 110.1(4) . .
O62 Ag2 Ag3 142.4(4) 2_645 3_756
S2 Ag2 Ag3 44.44(18) . 3_756
S1 Ag2 Ag3 107.9(2) . 3_756
O10 Ag2 Ag3 105.3(4) . 3_756
Ag1 Ag2 Ag3 54.58(6) . 3_756
O62 Ag2 Ag4 67.9(4) 2_645 .
S2 Ag2 Ag4 40.79(18) . .
S1 Ag2 Ag4 121.85(18) . .
O10 Ag2 Ag4 129.9(4) . .
Ag1 Ag2 Ag4 109.93(10) . .
Ag3 Ag2 Ag4 75.65(9) 3_756 .
O42 Ag3 S2 127.0(5) 2_745 3_756
O42 Ag3 S1 83.8(5) 2_745 .
S2 Ag3 S1 149.0(3) 3_756 .
O42 Ag3 Ag1 134.2(5) 2_745 .
S2 Ag3 Ag1 96.5(2) 3_756 .
S1 Ag3 Ag1 52.83(17) . .
O42 Ag3 Ag2 154.7(5) 2_745 3_756
S2 Ag3 Ag2 45.5(2) 3_756 3_756
S1 Ag3 Ag2 105.47(18) . 3_756
Ag1 Ag3 Ag2 53.22(6) . 3_756
O1W Ag4 S2 136.6(7) . .
O1W Ag4 O25 89.9(7) . 2_645
S2 Ag4 O25 103.7(4) . 2_645
O1W Ag4 O46 75.0(8) . 3_756
S2 Ag4 O46 130.9(5) . 3_756
O25 Ag4 O46 114.4(6) 2_645 3_756
O1W Ag4 Ag2 99.2(7) . .
S2 Ag4 Ag2 42.4(2) . .
O25 Ag4 Ag2 86.6(4) 2_645 .
O46 Ag4 Ag2 157.8(4) 3_756 .
O60 Ag5 O50 81.8(7) . 2_745
O60 Ag5 O2W 143.6(7) . .
O50 Ag5 O2W 110.9(7) 2_745 .
O60 Ag5 O15 99.8(6) . 2_645
O50 Ag5 O15 83.8(6) 2_745 2_645
O2W Ag5 O15 115.1(6) . 2_645
O60 Ag5 Ag10 115.8(6) . 3_655
O50 Ag5 Ag10 135.9(6) 2_745 3_655
O2W Ag5 Ag10 32.7(6) . 3_655
O15 Ag5 Ag10 127.5(6) 2_645 3_655
O3W Ag6 O2W 143.9(8) . .
O3W Ag6 O4W 98.3(7) . .
O2W Ag6 O4W 91.9(7) . .
O3W Ag6 O49 129.5(7) . 2_745
O2W Ag6 O49 84.2(6) . 2_745
O4W Ag6 O49 92.1(7) . 2_745
O3W Ag6 Ag10 39.6(6) . .
O2W Ag6 Ag10 107.1(7) . .
O4W Ag6 Ag10 87.6(7) . .
O49 Ag6 Ag10 168.7(6) 2_745 .
O3W Ag6 Ag10 119.0(6) . 3_655
O2W Ag6 Ag10 27.2(6) . 3_655
O4W Ag6 Ag10 86.0(6) . 3_655
O49 Ag6 Ag10 110.9(5) 2_745 3_655
Ag10 Ag6 Ag10 80.4(7) . 3_655
O54 Ag7 O3W 120.5(7) . .
O54 Ag7 O20 78.6(6) . 4_565
O3W Ag7 O20 89.5(6) . 4_565
O54 Ag7 Ag10 91.0(7) . .
O3W Ag7 Ag10 34.3(6) . .
O20 Ag7 Ag10 65.0(5) 4_565 .
O54 Ag7 Ag8 152.8(5) . 2_745
O3W Ag7 Ag8 47.3(4) . 2_745
O20 Ag7 Ag8 77.3(4) 4_565 2_745
Ag10 Ag7 Ag8 67.5(5) . 2_745
O13 Ag8 O3W 110.3(7) 4_666 2_755
O13 Ag8 O40 93.4(6) 4_666 .
O3W Ag8 O40 83.0(6) 2_755 .
O13 Ag8 O6W 77.3(7) 4_666 .
O3W Ag8 O6W 159.9(8) 2_755 .
O40 Ag8 O6W 77.9(6) . .
O13 Ag8 Ag7 155.7(5) 4_666 2_755
O3W Ag8 Ag7 46.2(5) 2_755 2_755
O40 Ag8 Ag7 79.0(4) . 2_755
O6W Ag8 Ag7 122.6(6) . 2_755
O5W Ag9 O2W 162.7(18) . .
O5W Ag9 O17 95.5(11) . 2_645
O2W Ag9 O17 83.5(7) . 2_645
O5W Ag9 Ag10 135.9(17) . 3_655
O2W Ag9 Ag10 31.8(6) . 3_655
O17 Ag9 Ag10 108.1(6) 2_645 3_655
O2W Ag10 O3W 171.5(17) 3_655 .
O2W Ag10 Ag6 136.5(13) 3_655 .
O3W Ag10 Ag6 51.6(7) . .
O2W Ag10 Ag9 40.7(9) 3_655 3_655
O3W Ag10 Ag9 139.5(11) . 3_655
Ag6 Ag10 Ag9 129.8(8) . 3_655
O2W Ag10 Ag5 44.7(8) 3_655 3_655
O3W Ag10 Ag5 128.3(12) . 3_655
Ag6 Ag10 Ag5 143.2(7) . 3_655
Ag9 Ag10 Ag5 76.7(5) 3_655 3_655
O2W Ag10 Ag7 133.3(11) 3_655 .
O3W Ag10 Ag7 45.9(8) . .
Ag6 Ag10 Ag7 74.3(5) . .
Ag9 Ag10 Ag7 93.6(6) 3_655 .
Ag5 Ag10 Ag7 136.0(8) 3_655 .
O2W Ag10 Ag6 37.7(8) 3_655 3_655
O3W Ag10 Ag6 149.2(11) . 3_655
Ag6 Ag10 Ag6 99.6(7) . 3_655
Ag9 Ag10 Ag6 65.0(5) 3_655 3_655
Ag5 Ag10 Ag6 66.0(4) 3_655 3_655
Ag7 Ag10 Ag6 147.1(8) . 3_655
W5 O1 W3 151.6(9) . .
P1 O2 W6 127.8(8) . .
P1 O2 W8 127.4(9) . .
W6 O2 W8 90.7(6) . .
P1 O3 W5 128.0(9) . .
P1 O3 W1 128.1(10) . .
W5 O3 W1 90.9(5) . .
P1 O4 W4 124.3(8) . .
P1 O4 W2 125.2(8) . .
W4 O4 W2 92.2(6) . .
P1 O4 W3 124.9(10) . .
W4 O4 W3 90.3(5) . .
W2 O4 W3 89.4(5) . .
P1 O5 W9 128.2(9) . .
P1 O5 W7 127.6(10) . .
W9 O5 W7 89.9(5) . .
P2 O6 W13 125.3(9) . .
P2 O6 W17 123.7(8) . .
W13 O6 W17 90.6(6) . .
P2 O6 W14 124.8(9) . .
W13 O6 W14 91.0(5) . .
W17 O6 W14 91.1(6) . .
P2 O7 W12 128.2(9) . .
P2 O7 W15 127.3(9) . .
W12 O7 W15 90.4(5) . .
P2 O8 W18 127.9(10) . .
P2 O8 W16 126.4(9) . .
W18 O8 W16 90.3(5) . .
P2 O9 W10 128.3(10) . .
P2 O9 W11 127.8(9) . .
W10 O9 W11 90.7(5) . .
W5 O10 W1 122.1(8) . .
W5 O10 Ag2 110.2(8) . .
W1 O10 Ag2 121.0(8) . .
W1 O11 W2 150.9(10) . .
W2 O13 Ag8 154.8(10) . 4_465
W3 O14 W2 125.5(8) . .
W3 O15 W4 123.2(8) . .
W3 O15 Ag5 110.2(8) . 2_655
W4 O15 Ag5 114.9(7) . 2_655
W4 O16 W2 123.6(10) . .
W3 O17 Ag9 115.9(10) . 2_655
W9 O18 W3 153.7(9) . .
W5 O19 W9 150.2(11) . .
W9 O20 Ag7 142.6(9) . 4_566
W7 O21 W4 151.2(9) . .
W9 O22 W7 123.0(8) . .
W10 O24 W9 165.3(9) . .
W4 O25 W8 150.1(11) . .
W4 O25 Ag4 110.9(8) . 2_655
W8 O25 Ag4 98.4(6) . 2_655
W6 O26 W2 152.3(11) . .
W18 O27 W5 162.8(10) . .
W1 O28 W16 162.9(11) . .
W1 O31 W6 152.0(10) . .
W16 O32 W18 123.4(9) . .
W10 O33 W18 153.9(10) . .
W8 O34 W6 122.5(10) . .
W8 O35 W12 164.6(10) . .
W10 O36 W11 121.9(9) . .
W8 O38 W7 153.8(9) . .
W11 O39 W7 160.7(10) . .
W10 O40 Ag8 146.1(9) . .
W12 O42 Ag3 175.5(11) . 2_755
W13 O43 W11 151.5(10) . .
W11 O44 W12 151.3(10) . .
W17 O45 W10 150.0(9) . .
W17 O46 Ag4 107.9(8) . 3_756
W15 O47 W12 124.0(8) . .
W12 O48 W13 150.3(10) . .
W13 O49 W17 121.0(9) . .
W13 O49 Ag6 118.3(7) . 2_755
W17 O49 Ag6 106.2(8) . 2_755
W13 O50 Ag5 133.9(10) . 2_755
W13 O51 W14 123.5(9) . .
W17 O52 W14 123.2(9) . .
W15 O54 Ag7 163.5(11) . .
W14 O55 W16 150.7(10) . .
W16 O56 W15 153.9(11) . .
W14 O58 W15 151.7(10) . .
W17 O59 W18 151.4(10) . .
W1 O60 Ag5 148.5(10) . .
W15 O61 W6 165.4(10) . .
W4 O62 Ag2 157.3(9) . 2_655
C3 S1 Ag1 114.6(10) . .
C3 S1 Ag2 99.6(10) . .
Ag1 S1 Ag2 72.02(19) . .
C3 S1 Ag3 105.3(10) . .
Ag1 S1 Ag3 72.6(2) . .
Ag2 S1 Ag3 142.8(3) . .
C8 S2 Ag4 113.2(10) . .
C8 S2 Ag3 111.4(10) . 3_756
Ag4 S2 Ag3 129.4(3) . 3_756
C8 S2 Ag2 109.0(11) . .
Ag4 S2 Ag2 96.9(3) . .
Ag3 S2 Ag2 90.1(3) 3_756 .
N1 C1 C2 120(3) . .
N1 C1 H1 119.9 . .
C2 C1 H1 119.9 . .
C3 C2 C1 117(3) . .
C3 C2 H2 121.4 . .
C1 C2 H2 121.4 . .
C2 C3 C4 122(3) . .
C2 C3 S1 117(2) . .
C4 C3 S1 121(2) . .
C5 C4 C3 119(3) . .
C5 C4 H4 120.5 . .
C3 C4 H4 120.5 . .
N1 C5 C4 117(3) . .
N1 C5 H5 121.6 . .
C4 C5 H5 121.6 . .
N2 C6 C7 112(3) . .
N2 C6 H6 124.0 . .
C7 C6 H6 124.0 . .
C8 C7 C6 125(3) . .
C8 C7 H7 117.7 . .
C6 C7 H7 117.7 . .
C9 C8 C7 119(3) . .
C9 C8 S2 120(2) . .
C7 C8 S2 121(2) . .
C8 C9 C10 118(3) . .
C8 C9 H9 121.1 . .
C10 C9 H9 121.1 . .
N2 C10 C9 119(3) . .
N2 C10 H10 120.6 . .
C9 C10 H10 120.6 . .
C1 N1 C5 124(3) . .
C1 N1 H1A 117.8 . .
C5 N1 H1A 117.8 . .
C10 N2 C6 128(3) . .
C10 N2 H2A 116.2 . .
C6 N2 H2A 116.2 . .
Ag10 O2W Ag9 107.5(13) 3_655 .
Ag10 O2W Ag5 102.7(11) 3_655 .
Ag9 O2W Ag5 124.1(8) . .
Ag10 O2W Ag6 115.1(11) 3_655 .
Ag9 O2W Ag6 104.8(8) . .
Ag5 O2W Ag6 103.1(9) . .
Ag10 O3W Ag6 88.8(9) . .
Ag10 O3W Ag7 99.8(10) . .
Ag6 O3W Ag7 106.7(8) . .
Ag10 O3W Ag8 115.7(11) . 2_745
Ag6 O3W Ag8 150.3(8) . 2_745
Ag7 O3W Ag8 86.5(6) . 2_745
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O60 1.714(17) .
W1 O28 1.863(18) .
W1 O11 1.894(18) .
W1 O31 1.899(18) .
W1 O10 1.934(17) .
W1 O3 2.380(16) .
W2 O13 1.700(18) .
W2 O14 1.909(15) .
W2 O26 1.916(16) .
W2 O11 1.925(18) .
W2 O16 1.938(16) .
W2 O4 2.373(17) .
W3 O17 1.725(17) .
W3 O14 1.877(17) .
W3 O15 1.892(17) .
W3 O1 1.927(17) .
W3 O18 1.937(18) .
W3 O4 2.410(15) .
W4 O62 1.713(17) .
W4 O25 1.910(16) .
W4 O21 1.922(18) .
W4 O16 1.932(17) .
W4 O15 1.953(16) .
W4 O4 2.361(16) .
W5 O12 1.720(18) .
W5 O1 1.890(18) .
W5 O19 1.889(16) .
W5 O10 1.908(17) .
W5 O27 1.923(18) .
W5 O3 2.335(15) .
W6 O30 1.701(18) .
W6 O26 1.903(17) .
W6 O31 1.902(18) .
W6 O61 1.914(18) .
W6 O34 1.918(16) .
W6 O2 2.357(16) .
W7 O23 1.686(16) .
W7 O21 1.890(18) .
W7 O39 1.897(17) .
W7 O38 1.899(16) .
W7 O22 1.930(17) .
W7 O5 2.397(15) .
W8 O37 1.711(17) .
W8 O35 1.851(17) .
W8 O38 1.893(17) .
W8 O34 1.906(17) .
W8 O25 1.938(17) .
W8 O2 2.356(15) .
W9 O20 1.701(18) .
W9 O18 1.880(18) .
W9 O22 1.893(16) .
W9 O19 1.905(15) .
W9 O24 1.912(17) .
W9 O5 2.358(16) .
W10 O40 1.726(19) .
W10 O33 1.874(15) .
W10 O24 1.885(17) .
W10 O36 1.906(16) .
W10 O45 1.957(17) .
W10 O9 2.349(17) .
W11 O41 1.691(17) .
W11 O44 1.884(17) .
W11 O39 1.898(17) .
W11 O43 1.914(17) .
W11 O36 1.943(18) .
W11 O9 2.381(15) .
W12 O42 1.704(17) .
W12 O48 1.885(19) .
W12 O44 1.902(16) .
W12 O47 1.912(16) .
W12 O35 1.921(18) .
W12 O7 2.350(15) .
W13 O50 1.742(17) .
W13 O43 1.909(16) .
W13 O51 1.918(16) .
W13 O48 1.92(2) .
W13 O49 1.932(19) .
W13 O6 2.374(15) .
W14 O53 1.706(17) .
W14 O58 1.881(19) .
W14 O55 1.901(16) .
W14 O51 1.933(15) .
W14 O52 1.937(19) .
W14 O6 2.383(15) .
W15 O54 1.697(18) .
W15 O61 1.878(18) .
W15 O56 1.886(17) .
W15 O47 1.907(16) .
W15 O58 1.926(19) .
W15 O7 2.405(15) .
W16 O57 1.699(17) .
W16 O56 1.891(19) .
W16 O32 1.901(18) .
W16 O28 1.926(17) .
W16 O55 1.925(17) .
W16 O8 2.414(15) .
W17 O46 1.70(2) .
W17 O59 1.885(17) .
W17 O45 1.909(16) .
W17 O52 1.929(18) .
W17 O49 1.955(17) .
W17 O6 2.383(18) .
W18 O29 1.709(19) .
W18 O27 1.879(18) .
W18 O33 1.903(15) .
W18 O32 1.912(16) .
W18 O59 1.953(17) .
W18 O8 2.321(17) .
P1 O5 1.521(17) .
P1 O3 1.531(16) .
P1 O2 1.561(16) .
P1 O4 1.565(18) .
P2 O9 1.519(15) .
P2 O8 1.536(16) .
P2 O7 1.550(18) .
P2 O6 1.579(18) .
Ag1 S1 2.494(7) .
Ag1 S1 2.494(7) 3_756
Ag1 Ag2 2.936(3) .
Ag1 Ag2 2.936(3) 3_756
Ag1 Ag3 2.987(3) .
Ag1 Ag3 2.987(3) 3_756
Ag2 O62 2.432(18) 2_645
Ag2 S2 2.487(8) .
Ag2 S1 2.499(7) .
Ag2 O10 2.606(17) .
Ag2 Ag3 3.490(4) 3_756
Ag2 Ag4 3.665(5) .
Ag3 O42 2.408(17) 2_745
Ag3 S2 2.443(8) 3_756
Ag3 S1 2.550(8) .
Ag3 Ag2 3.490(4) 3_756
Ag4 O1W 2.24(2) .
Ag4 S2 2.412(8) .
Ag4 O25 2.701(19) 2_645
Ag4 O46 2.750(19) 3_756
Ag5 O60 2.297(19) .
Ag5 O50 2.41(2) 2_745
Ag5 O2W 2.42(2) .
Ag5 O15 2.457(16) 2_645
Ag5 Ag10 3.36(2) 3_655
Ag6 O3W 2.451(19) .
Ag6 O2W 2.48(2) .
Ag6 O4W 2.63(2) .
Ag6 O49 2.724(19) 2_745
Ag6 Ag10 3.12(2) .
Ag6 Ag10 3.68(2) 3_655
Ag7 O54 2.471(19) .
Ag7 O3W 2.54(2) .
Ag7 O20 2.758(19) 4_565
Ag7 Ag10 3.48(2) .
Ag7 Ag8 3.512(8) 2_745
Ag8 O13 2.393(19) 4_666
Ag8 O3W 2.587(18) 2_755
Ag8 O40 2.661(19) .
Ag8 O6W 2.68(3) .
Ag8 Ag7 3.512(8) 2_755
Ag9 O5W 2.06(4) .
Ag9 O2W 2.30(2) .
Ag9 O17 2.73(2) 2_645
Ag9 Ag10 3.36(2) 3_655
Ag10 O2W 1.86(3) 3_655
Ag10 O3W 1.99(3) .
Ag10 Ag9 3.36(2) 3_655
Ag10 Ag5 3.36(2) 3_655
Ag10 Ag6 3.68(2) 3_655
O13 Ag8 2.393(19) 4_465
O15 Ag5 2.457(16) 2_655
O17 Ag9 2.73(2) 2_655
O20 Ag7 2.758(19) 4_566
O25 Ag4 2.701(19) 2_655
O42 Ag3 2.408(17) 2_755
O46 Ag4 2.750(19) 3_756
O49 Ag6 2.724(19) 2_755
O50 Ag5 2.41(2) 2_755
O62 Ag2 2.432(18) 2_655
S1 C3 1.79(3) .
S2 C8 1.77(3) .
S2 Ag3 2.444(8) 3_756
C1 N1 1.31(4) .
C1 C2 1.41(4) .
C1 H1 0.9300 .
C2 C3 1.35(4) .
C2 H2 0.9300 .
C3 C4 1.41(4) .
C4 C5 1.39(4) .
C4 H4 0.9300 .
C5 N1 1.36(4) .
C5 H5 0.9300 .
C6 N2 1.34(3) .
C6 C7 1.41(4) .
C6 H6 0.9300 .
C7 C8 1.37(4) .
C7 H7 0.9300 .
C8 C9 1.34(4) .
C9 C10 1.45(4) .
C9 H9 0.9300 .
C10 N2 1.29(4) .
C10 H10 0.9300 .
N1 H1A 0.8600 .
N2 H2A 0.8600 .
O2W Ag10 1.86(3) 3_655
O3W Ag8 2.587(18) 2_745
